## Experimental Investigation of the Dynamic

## Characteristics of Laminated Composite Beams

### Mohammed F. Aly, I. G. M. Goda, and Galal A. Hassan

**Abstract**

**— **

**The laminated composite beams are basic**

**structural components used in a variety of engineering**

**structures such as airplane wings, helicopter blades and**

**turbine blades as well as many others in the aerospace,**

**mechanical, and civil industries. An important element in the**

**dynamic analysis of composite beams is the computation of**

**their natural frequencies and mode shapes. This is important**

**because composite beam structures often operate in complex**

**environmental conditions and are frequently exposed to a**

**variety of dynamic excitations. In this paper, a combined**

**finite element and experimental approach is used to**

**characterize the vibration behavior of composite beams. To**

**this end, some beams are made using the hand-lay-up**

**process. Glass fiber is used as reinforcement in the form of**

**bidirectional fabric and general purpose polyester resin as**

**matrix for the composite material of beams. Experimental**

**dynamic tests are carried out using specimens with different**

**fiber orientations. From the results, the influence of fiber**

**orientations on the flexural natural frequencies is**

**investigated. Also, these experiments are used to validate the**

**results obtained from the finite element software ANS YS .**

**Index Term**

**– **

**Composite beams, Dynamic tests, Finite**

**element method, Natural frequencies**

I. INTRODUCTION

Fiber reinforced composites are finding increasing applications in civil engineering, transportation vehicles, aerospace, marine, aviation, and chemical industries in recent decades. This is due to their excellent features, such as high strength-to-weight and stiffness -to-weight ratios, the ability of being different strengths in different directions and the nature of being tailored to satisfy the strength and stiffness requirements in practical designs. Studies on the behavior of composite beams have recently been important because of their high strength and lightweight properties on modern engineering sought in structures. For any composite structure that may be subjected to dynamic loads, the determination of the natural frequencies is critical in the design process. It is

Mohammed F. Aly is with the Department of Industrial Engineering, Fayoum University, Fayoum, Egypt. (Phone:

+20101692563), (email: mfahmy_aly@yahoo.com and mfa03@fayoum.edu.eg,).

I. G. M. Goda is with the Department of Industrial Engineering, Fayoum University, Fayoum, Egypt. (Phone: +20115838789), (email:

igm00@fayoum.edu.eg).

Galal A. Hassan is with the Department of Mechanical Design and Production, Cairo University, Cairo, Egypt. (Phone: +20103541315),

(email: galalhassaan@yahoo.com).

usually the first step in a dynamic analysis since a great deal may be deduced concerning the structural behavior and integrity from knowledge of its natural frequencies. So, the researches pertain to the vibration analysis of composite beams have undergone rapid growth over the past few decades and are still growing.

A number of researchers have been developed numerous solution methods to analysis the dynamic behavior of laminated composite beams. Khdeir and Reddy [[1]] developed analytical solutions of refined beam theories to study the free vibration behavior of cross -ply rectangular beams with arbitrary boundary conditions in conjunction with the state space approach. Krishnaswamy et al. [[2]] developed dynamic equations governing the free vibration of laminated composite beams using Hamilton's principle. The effects of transverse shear and rotary inertia are included in the energy formulation. Matsunaga [[3]] studied the natural frequencies of laminated composite beams by taking into account the complete effects of transverse shear and normal stresses and rotatory inertia. Chen et al. [[4]] presented a new method of state space-based differential quadrature for free vibration of generally laminated beams. Chandrashekhara et al. [[5]] obtained the exact solutions for symmetrically laminated beams based on first order shear deformation theory including rotary inertia.

analyze free and forced vibrations of non -uniform composite beams in the Laplace domain. Song and Waas [[12]] studied the free vibration analyses of stepped laminated composite beams using simple higher-order theory (SHOT) which assumes a cubic distribution for the displacement field through the thickness. Yildirim [[13]] used the stiffness method for the solution of the purely in-plane free vibration problem of symmetric cross -ply laminated beams with the rotary inertia, axial and transverse shear deformation effects included by the first -order shear deformation theory. Rao et al. [[14]] developed an analytical method for evaluating the natural frequencies of laminated composite and sandwich beams using higher-order mixed theory and analyzed various beams of thin and thick sections. Kant et al. [[15]] developed an analytical solution to the dynamic analysis of the laminated composite beams using a higher order refined theory. Vinson and Sierakowski [[16]] obtained the exact solution of a simply supported composite beam based on the classical theory, which neglects the effects of the rotary inertia and shearing deformation. Abramovich [[17]] studied free vibration of symmetrically laminated composite beams on Timoshenko type equations.

Many authors have used the finite element technique to analyze the dynamic of laminated beams. Bassiouni et al. [[18]] presented a finite element model to investigate the natural frequencies and mode shapes of the laminated composite beams. Tahani [[19]] developed a new layerwise beam theory for generally laminated composite beam and compared the analytical solutions for static bending and free vibration with the three-dimensional elasticity solution of cross -ply laminates in cylindrical bending and with three-dimensional finite element analysis for angle-ply laminates. Chandrashekhara and Bangera [[20]] investigated the free vibration of angle-ply composite beams by a higher-order shear deformation theory using the shear flexible finite element method. Maiti and Sinha [[21]] developed a finite element method (FEM) to analyze the vibration behavior of laminated composite. Murthy et al. [[22]] derived a refined 2-node beam element based on higher order shear deformation theory for axial-flexural-shear coupled deformation in asymmetrically stacked laminated composite beams. Ramtekkar et al. [[23]] developed a six-node plane-stress mixed finite element model by using Hamilton’s principle. Teh and Huang [[24]] presented two finite element models based on a first-order theory for the free vibration analysis of fixed-free beams of general orthotropy. Nabi and Ganesan [[25]] developed a general finite element based on a first-order deformation theory to study the free vibration characteristics of laminated composite beams. Aydogdu [[26]] studied the vibration of cross -ply laminated beams subjected to different sets of boundary conditions. Subramanian [[27]] has investigated the free vibration of laminated composite beams by using two higher order displacement based on shear deformation theories and finite elements.

The main objective of this work is to contribute for a better understanding of the dynamic behavior of

components made from fiber reinforced composite materials, specifically for the case of beams. In order to investigate the influence of the fiber orientation on the dynamic behavior of the components, experimental and numerical analysis using the finite element method have been carried out. The results are presented and discussed.

II. PRODUCTION OF THE LAM INATES SPECIM ENS Glass fiber is used as reinforcement in the form of bidirectional fabric and general purpose polyester resin as matrix for the composite material of the laminates specimens.

The steps of manufacturing the composite beams using the hand lay-up process are described below.

**A.****Preparation of the Mould **

The hand lay-up process is open molding technique, only one mould is used. The surface of the mould is thoroughly cleaned to be ready for the use, by removing any dust and dirt from it.

**B.****Application of the Release Agent**** **

After the mould surface has been cleaned, the release agent is applied. Where, the mould surface is coated with a silicon free wax using a smooth cloth. Then a film of polyvinyl alcohol (PVA) is applied over the wax surface using sponge. PVA is a water soluble material and 15% solution in water is used. When water evaporates, a thin film of PVA is formed on the mould surface. PVA film is dried completely before the application of resin coat. This is very important as the surface of final article will be marred with a partly dried PVA film otherwise release will not be smooth.

**C.****Preparation of the Matrix Material **

The matrix material is prepared using General purpose (GP) Polyester resin. Cobalt Octate (0.35% by volume of resin) is added to act as Accelerator. Methyl ethyl ketone peroxide (MEKP) (1% by volume) is added to act as catalyst. Resin, accelerator and catalyst are thoroughly mixed. The use of accelerator is necessary because without accelerator resin does not cure properly. After adding the accelerator and catalyst to the polyester resin, it has left for some time so that bubbles formed during stirring may die out. The amount of added accelerator and catalyst is not high because a high percentage reduces gel time of polyester resin and may adversely affect impregnation.

**D.****Preparation of the Reinforcement **

Fig. 1. Schematic representation of woven fabric architecture [ [28]]

**E.****Preparation of the Laminated Plate **

The first layer of mat is laid and resin is spread uniformly over the mat by means of a brush. The second layer of mat is laid and resin is spread uniformly over the mat by means of a brush. After second layer, to enhance wetting and impregnation, a teethed steel roller is used to roll over the fabric before applying resin. Also resin is tapped and dabbed with spatula before spreading resin over fabric layer. This process is repeated till all the twelve fabric layers are placed. No external pressure is applied while casting or curing because uncured matrix material can squeeze out under high pressure. This results in surface waviness (non-uniform thickness) in the model material. The casting is cured at room temperature for 4 hours and finally removed from the mould to get a fine finished composite plate.

**F.****Preparation of the Test Specimens **

After the cure process, test specimens are cut from the sheet of 12 ply laminate of the size 1000 mm x 1000 mm x 5.45 mm by using a diamond impregnated wheel, cooled by running water. All the test specimens are finished by abrading the edges on a fine carborundum paper.

The laminated plate is cut at different off-axis angles (00, 150, and 300) to give beam specimens with different fiber orientation of twelve woven lamina. Since each fabric layer corresponds to 2 different fiber orientations (fibers at 00 and 900) 2 different layers can be used to simulate each ply as ([0/90], [15/-75], and [30/-60]).

III. MATERIALS AND EXPERIM ENTAL TEST SPECIM ENS

**A.****Materials Characterization **

The mechanical properties of constituents of the test specimens, E-glass woven roving fibers and polyester matrix are listed in Table 1.

The material elastic properties of the laminae of test
specimens are determined through the simple
rule-of-mixtures. These properties are Young’s moduli (*E1* – in
direction 1, *E2* – in direction 2, *E3* – in direction 3),
Poisson’s ratios (*ν12*, *ν13*, and *ν23* ), Inplane shear modulus
(*G12*) and transverse shear moduli (*G13* and *G23*) as referred
in Fig.2. This figure defines the material principal axes for
a typical woven fiber reinforced lamina. Axis 1 is along
the fiber length and represents the longitudinal direction of

the lamina; axes 2 and 3 represent the transverse in -plane and through- the- thickness directions respectively.

TABLE I

MECHANICAL PROPERT IES OF CONST IT UENT S OF T EST SPECIMENS [[29]]

**Material ** **Properties ** **Value **

**Glass fiber **

Elasticity modulus (GPa) 74

Shear modulus (GPa) 30

Density (kg/m3) 2600

Poisson ratio 0.25

**Polyester **
**resin**

Elasticity modulus (GPa) 4.0

Shear modulus (GPa) 1.4

Density (kg/m3) 1200

Poisson ratio 0.4

Fig. 2. Lamina reference axes

The volume fractions of the fiber and voids are calculated from the measured weights and densities of fiber, matrix, and composite. The fiber weight fraction of the specimens is measured by burning out the resin of the composite material. In the burning test, three samples have nominal 5.45 mm thicknesses are cut in square sections of 43×43 mm. An electronic balance is used to measure the weight of the three samples of the tested woven fabric composite. The averaged weight of the three samples is measured as 16.48 gm. The average density of the samples is found to be 1610 kg/m3. After the burning process, the resin is removed from the composite and the average weighted of the remaining woven roving fiber becomes 7.55 gm. Then, the fiber weight fraction of the composite material is calculated to be 45.83% and the resin weight fraction is 54.17%.

*c*
*c*
*m*
*f*
*c*
*f*
*f*

*W*

*W*

*W*

*W*

###

###

###

###

_{}

### /

### /

### )

### (

### )

### /

### (

### 1

###

###

###

###

(1)Where *Wf,Wm*, and *Wc* are the weights of the fiber, matrix,
and composite, respectively.

By using the densities of the fiber* ρf*, matrix* ρm*, and
composite* ρc*, respectively, the fiber volume fraction *υf* can
be obtained by equation (2):

) 1 (

###

###

_{}

###

###

###

###

###

###

###

###

**

_{c}

_{f}**

_{f}

_{m}**

_{m}

_{f}**

_{f}**

_{m}* (2)*

_{f}Where *νf*, *νm*, and *νυ* are the volume fractions of the fiber,
matrix, and voids, respectively.

Using the relation of equation (2) the fiber volume fraction
(*νf* ) is found 30 % according to the densities of fiber and
matrix presented in Table 1. Then, the elastic constants of
the woven fabric composite material are numerically
estimated using the relations which are based on their
constituent properties. The young's modulus and the
Poisson's ratio of the fill and warp directions are calculated
and taken as an average of the longitudinal and transverse
values of the corresponding unidirectional layer.

The elastic constants of the unidirectional composite are calculated using the simple rule-of-mixtures by the relations of equation (3) [[16]].

.
)
1
(
2
,
)
(
)
(
,
/
1
/
1
)
1
(
),
1
(
,
)
(
)
(
),
1
(
23
22
23
12
11
12
2
11
12
23
12
2
1
*E*
*G*
*G*
*G*
*G*
*G*
*G*
*G*
*G*
*G*
*G*
*G*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*f*
*m*
*f*
*m*
*f*
*f*
*m*
*f*
*m*
*f*
*m*
*m*
*m*
*m*
*m*
*m*
*f*
*m*
*f*
*f*
*f*
*m*
*f*
*f*
*f*
*m*
*f*
*m*
*f*
*f*
*m*
*f*
*m*
*f*
*m*
*f*
*m*
*f*
*f*
(3)

Where indices *m* and *f* denote matrix and fiber,
respectively

After calculating elastic constants of the unidirectional composite, elastic constants of the woven fabric composite material are estimated using the relations of equation (4) [[28]] and the results are listed in Table 2.

.
1
2
1
1
,
1
1
,
1
)
)
2
1
(
(
)
2
2
1
(
)
1
(
,
)
2
1
(
)
(
1
,
)
2
1
(
)
2
(
)
(
4
,
1
)
2
1
(
)
2
(
)
)
1
(
(
2
13
12
2
23
12
12
3
2
12
1
2
1
2
2
2
12
2
1
23
12
12
2
1
2
23
1
13
2
12
1
2
2
12
23
12
23
12
1
1
1
12
2
2
2
12
2
1
1
2
2
12
1
2
12
1
1
2
2
2
12
2
1
1
2
2
2
12
2
2
12
1
1
1
*WF*
*UD*
*WF*
*UD*
*WF*
*UD*
*WF*
*UD*
*WF*
*UD*
*WF*
*UD*
*G*
*G*
*E*
*G*
*G*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
*E*
(4)

Where *UD* and *WF* denote unidirectional fiber and woven
fiber, respectively

TABLE II

ELAST IC PROPERT IES OF WOVEN FABRIC COMPOSIT E LAMINAE

**Properties ** **Value **

Elastic modulus *E1* = *E2* (GPa) 15.70

Elastic modulus *E3* (GPa) 7.85

Shear modulus in plane 1–2 *G12* (GPa) 2.45

Shear modulus in plane 1–3 *G13* (GPa) 2.37

Shear modulus in plane 2–3 *G23* (GPa) 2.37

Poisson ratio in plane 1–2 *υ12* 0.15

Poisson ratio in plane 1–3 *υ13* 0.46

Poisson ratio in plane 2–3 *υ23* 0.46

**B.****Types of Structures **

All types of structures investigated in this study are in the form of simple beams. The laminate is cut in beams with nominal length of 370 mm, width of 43 mm, thickness of 5.45 mm, and total mass equal to 140 gm. The types of lay up of beams under investigation are varied as 00, 150, and 300 as shown in Fig.3. The total length of the beam specimens is 370 mm and due to the cantilevered fixation of the test specimens the free length becomes 330 mm.

**C.****Experimental Modal Analysis **

Through an impact experimental test, it is determined FRFs (Frequency Response Functions) which relate the response given by the specimen when loaded with a signal, allowing for the determination of the natural frequencies, as shown in Fig.4. This is done by fixing the laminate specimen in a rigid support with one of its side free to vibrate, as a cantilever beam. The impact hammer is used to give the input load (pulse) to the specimen, and the Signal Analyzer is set from 0 Hz to 200 Hz. This output is captured by the accelerometer and is amplified using a conditioning amplifier and then read using the high resolution signal analyzer, giving the FRF.

1- Cantilever laminated beam 2- B&K accelerometer Type 4333

3- B&K conditioning amplifier Type 2626 4- B&K signal analyzer Type 2033

Fig. 4. Experimental set up for modal testing of a cantilever laminated beam

IV. RESULTS AND DISCUSSIONS

Table 3 shows the experimental damped natural frequencies obtained by free vibration test for all laminated beams previously mentioned. Figs. 5-7 present the 1st and 2nd natural frequencies obtained experimentally for the woven laminated beam of fiber angle 00, 150, and 300.

Also, theses beams are modeled using finite element
method in order to get the un-damped natural frequencies
and mode shapes. The beams are discretized using (type
shell99) finite element available in the commercial
package ANSYS 10.0. This element has 8 nodes and is
constituted by layers that are designated by numbers (LN -
Layer Number), increasing from bottom to top of the
laminate. The last number quantifies the existent total
number of layers in the laminate (NL - Total Number of
Layers). The element has six degrees of freedom at each
node: translations in the nodal *x*, *y*, and *z* directions and
rotations about the nodal *x*, *y*, and *z*-axes.

The constituent laminae are considered to be linear elastic and generally orthotropic therefore the concept of engineering constants is used to describe the laminae elastically. The elastic properties of the woven roving laminae are required as input parameters for the ANSYS.

These properties are E1, E2, E3, G12, G13, G23, υ12, υ13 and υ23 which are given in Table II. The results obtained by ANSYS are presented in Table III, for the first two un-damped natural frequencies.

TABLE III

NAT URAL FREQUENCIES (HZ) FROM ANSYS AND EXPERIMENT AL T EST

**Lay **

**up **

**1st mode ** **2nd mode **

**Ansys ** **Exp. ** **% Diff. Ansys ** **Exp. ** **% Diff. **

**0 ** 25.1 22.0 12.4 157.0 146.5 6.7

**15 ** 22.7 20.0 11.9 141.8 143.5 1.2

**30 ** 19.48 17.0 12.7 121.7 121.0 0.6

100

%

*ANSYS*
*al*
*Experiment*
*ANSYS*

*f*
*f*
*f*

*Difference*

From the results of Table III, it has been found that the experimental results show a good agreement with the ANSYS values (maximum difference equal 12.7 % for the 1st mode and 6.7 % for the 2nd mode), proving that the fiber angle has influence on the dynamic behavior of the laminated beams. As the fiber angle increases, the natural frequencies of flexural vibration of beams decrease. From the experimental results, it is observed that increasing the angle of the fibers from 00 to 300 reduces the natural frequency by about 23% (i.e. from 22 to 17 Hz) for the 1st mode and by about 17.5% (i.e. from 146.5 to 121.0 Hz) for the 2nd mode.

From these results, it is possible to verify the
influence of fiber orientation on the free flexural vibration
of laminated beams. It is found that the maximum flexural
frequency occurs at *β* = 00 and the minimum occurs at 300.
This can be explained by the fact that the fibers oriented at
00 are more appropriate to flexural loads

Fig. 6. 1st and 2nd flexural frequencies obtained by experimental dynamic
test for 150_{ woven roving laminated beam}

Fig. 7. 1st and 2nd flexural frequencies obtained by experimental dynamic test for 300 woven roving laminated beam

Variation of the lowest two flexural frequencies with respect to fiber angle change of woven roving laminated beams are presented in Fig. 8. The experimental frequencies are plotted with the ANSYS results against fiber angle of woven roving laminated beams.

**0**
**20**
**40**
**60**
**80**
**100**
**120**
**140**
**160**
**180**

**0** **5** **10** **15** **20** **25** **30** **35** **40** **45**

**Fiber angle (degree)**

**N**

**a**

**tu**

**ra**

**l **

**fr**

**e**

**q**

**u**

**e**

**n**

**c**

**y**

** (**

**H**

**z)**

**1st Mode (ANSYS)**
**2nd Mode (ANSYS)**
**1st Mode (Experimental)**
**2nd Mode (Experimental)**

Fig. 8. Variation of 1st_{ and 2}nd_{ flexural frequencies with respect to }

fiber angle change of woven roving laminated beams

With relation to the deviations of the numerical results in relation to the experimental ones, some possible measurement errors can be pointed out such as: measurement noise, positioning of the accelerometers and their mass, non-uniformity in the specimens properties (voids, variations in thickness, non uniform surface finishing). Such factors are not taken into account during the numerical analysis, since the model considers the specimen entirely perfect and with homogeneous properties, what rarely occurs in practice. Another aspect to be considered is that the input properties in the model came from the application of the rule-of-mixtures and they do not take into account effects of the fiber-matrix interface as well as the irregular distribution of resin on the fibers. Also, these models did not include damping effects, which can have a large influence on the structure behavior. Also, the computational package ANSYS does not allow for the consideration of the fibers interweaving present in the fabric used.

The mode shapes associated with the frequencies of 00 woven roving beam are illustrated in Fig. 9. They are deduced by ANSYS for the first and second flexural natural frequencies (deformed and un-deformed shapes).

X

Y

Z

APR 17 2009

02:55:19

1st_{ Mode - 25.1 Hz}
1

X Y

Z

APR 17 2009

02:55:32 DISPLACEMENT

2nd Mode – 157.0 Hz

Fig. 9. Free flexural modes for 00 woven roving beam

V. CONCLUSIONS

In this work, the dynamic characteristics of laminated composite beams with different fiber orientations were tested experimentally. The test results were compared to those calculated using finite element software package ANSYS. The main conclusions that can be drawn from this investigation are:

The changes in fiber angle yield to different dynamic behavior of the component, that is, different natural frequencies for the same geometry, mass and boundary conditions.

As the fiber angle increases, the flexural natural
frequencies decrease, with maximum value
occurs at *β* = 00.

The results from ANSYS showed in general good agreement with the experimental values.

The experimental investigation conducted using specially prepared beam specimens with different fiber orientations was reasonable.

The numerical analysis using finite element package ANSYS to investigate the dynamic characteristics of laminated composite beams, is a successful tool for such applications.

Finally, this study helps designer in selection of the fiber orientation angle to shift the natural frequencies as desired or to control the vibration level.

REFERENCES

[1] Khdeir, A.A., and Reddy, J.N., "Free vibration of cross-ply laminated beams with arbitrary boundary conditions", International Journal of Engineering Science, Vol. 32, 1994, pp.1971 -1980.

[2] Krishnaswamy, S., Chandrashekhara, K., and Wu, W.Z., "Analytical solutions to vibration of generally layered composite beams", Journal of Sound and Vibration, Vol. 159, 1992, pp. 85-99. [3] Matsunaga, H., "Vibration and buckling of multilayered composite beams according to higher order deformation theories", Journal of Sound and Vibration, Vol. 246, 2001, pp.47 -62.

[4] Chen, W.Q., Lv, C.F., and Bian, Z.G., "Free vibration analysis of generally laminated beams via state-space-based differential quadrature", Composite Structures, Vol. 63, 2004, PP. 417 -425. [5] Chandrashekhara, K., Krisnamurty, K., and Roy S., "Free vibration of composite beams including rotary inertia and shear deformation", Composite Structures, Vol. 14, 1990, PP. 269 -279.

[6] Yildirim, V., and Kiral, E., "Investigation of the rotary inertia and shear deformation effects on the out -of-plane bending and torsional natural frequencies of laminated beams", Composite Structures, Vol.49, 2000, pp. 313-320.

[7] Banerjee, J.R., "Free vibration of axially loaded composite timoshenko beams using the dynamic stiffness matrix method", Computers and Structures, Vol. 69, 1998, pp. 197 -208. [8] Jun, L., Hongxing, H., and Rongying, S., "Dynamic stiffness

analysis for free vibrations of axially loaded laminated composite beams", Composite Structures, Vol. 84, 2008, pp. 87 -98. [9] Abramovich, A., and Livshits, A., "Free vibration of non -symmetric

cross-ply laminated composite beams", Journal of Sound and Vibration, Vol. 38, 1994, pp. 597 -612.

[10] Eisenberger, M., Abramovich, H., and Shulepov, O., "Dynamic stiffness analysis of laminated beams using a first -order shear deformation theory", Composite Structure, Vol. 31, 1995, pp. 265-271.

[11] Calım, F.F., "Free and forced vibrations of non-uniform composite beams", Composite Structures, 2008.

[12] Song, S.J., and Waas A.M., "Effects of shear deformation on buckling and free vibration of laminated composite beams", Composite Structures, Vol.37, 1997, pp .33-43.

[13] Yildirim, V., "Effect of the longitudinal to transverse moduli ratio on the in-plane natural frequencies of symmetric cross-ply laminated beams by the stiffness method" Composite Structures, Vol.50, 2000, pp. 319-326.

[14] Rao, M.K., Desai, Y.M., and Chitnis, M.R., "Free vibrations of laminated beams using mixed theory", Composite Structures, Vol. 52, 2001, pp. 149-160.

[15] Kant, T ., Marurb, S.R., and Rao, G.S., "Analytical solution to the dynamic analysis of laminated beams using higher order refined theory", Composite Structures, Vol.40, 1998, pp. 1 -9. [16] Vinson, J.R., and Sierakowski, R.L., T he behaviour of structures

composed of composite materials, New York, Boston, Dordrecht, Moscow, 2004.

[17] Abramovich, H., "Shear deformations and rotary inertia effects of vibrating composite beams", Composite Structures, Vol. 20, 1992, pp. 165-173.

[18] Bassiouni, A.S., Gad-Elrab, R.M., and Elmahdy T .H., "Dynamic analysis for laminated composite beams", Composite Structures, Vol. 44, 1999, pp. 81-87.

[19] T ahani, M., "Analysis of laminated composite beams using layerwise displacement theories", Composite Structures, Vol.79, 2007, pp.535-547.

[20] Chandrashekhara, K., and Bangera, K.M., "Free vibration of composite beams using a refined shear flexible beam element", Computer and Structures, Vol. 43, 1992, pp. 719-727. [21] Maiti, D.K., and Sinha, P.K., "Bending and free vibration analysis

of shear deformable laminated composite beams by finite element method", Composite Structures, Vol.29, 1994, pp. 421 -431. [22] Murthy, M.V., Mahapatra, D.R., Badarinarayana, K., and

Gopalakrishnan, S., "A refined higher order finite element for asymmetric composite beams", Composite Structures, Vol.67, 2005, pp. 27-35.

[23] Ramtekkar, G.S., Desai, Y.M., and Shah, A.H., "Natural vibrations of laminated composite beams by using mixed finite element modeling", Journal of Sound and Vibration, Vol.257, 2002, pp. 635-651.

[25] Nabi, M.S., and Ganesan, N., "A generalized element for the free vibration analysis of composite beams", Computer and Structures, Vol.51, 1994, pp. 607-610.

[26] Aydogdu, M., "Vibration analysis of cross-ply laminated beams with general boundary conditions by Ritz method", International Journal of Mechanical Sciences, Vol.47, 2005, pp. 1740 -1755. [27] Subramanian, P., "Dynamic analysis of laminated composite beams using higher order theories and finite elements", Composite Structures, Vol. 73, 2006, pp. 342-353.

[28] Akkerman, R., "Laminate mechanics for balanced woven fabrics", Composites, Vol.37, 2006, PP. 108 -116.